Significance and Use
4.1 Personnel utilizing reference radiographs to this standard shall be qualified and authorized to perform radiographic interpretation in accordance with a nationally or internationally recognized NDT personnel qualification practice or standard such as ANSI/ASNT-CP-189, SNT-TC-1A, NAS 410, ISO 9712, or a similar document and certified by the employer or certifying agency, as applicable. The practice or standard used and its applicable revision shall be identified in the contractual agreement between the using parties. A certified Level III shall be available to assist with interpreting specifications and product requirements as applied to the reference radiographs (if the Level III is the radiographic interpreter, this may be the same person).
4.2 Graded reference radiographs are intended to provide a guide enabling recognition of specific casting discontinuity types and relative severity levels that may be encountered during typical fabrication processes. Reference radiographs containing ungraded discontinuities are provided as a guide for recognition of a specific casting discontinuity type where severity levels are not needed. These reference radiographs are intended as a basis from which manufacturers and purchasers may, by mutual agreement, select particular discontinuity classes to serve as standards representing minimum levels of acceptability (see Sections and ).
4.3 Reference radiographs represented by this standard may be used, as agreed upon in a purchaser supplier agreement, for energy levels, thicknesses, or both, outside the range of this standard when determined applicable for the casting service application. Severity levels of similar discontinuity categories and energy level range of Reference Radiographs reference radiographs may alternatively be used, as determined appropriate for the casting service application, if so agreed upon in the purchaser supplier agreement (see and ).
4.4 Procedures for evaluation of production radiographs using applicable reference radiographs of this standard are prescribed in Section ; however, there may be manufacturing-purchaser issues involving specific casting service applications where it may be appropriate to modify or alter such requirements. Where such modifications may be appropriate for the casting application, all such changes shall be specifically called-out in the purchaser supplier agreement or contractual document. Section addresses purchaser supplier requisites for where weld repairs may be required.
1.1 These reference radiographs illustrate various categories, types, and severity levels of discontinuities occurring in steel castings that have section thicknesses up to 2 in. (50.8 mm) (see ). The reference radiograph films are an adjunct to this standard and must be purchased separately from ASTM International, if needed (see ). Categories and severity levels for each discontinuity type represented by these reference radiographs are described in .
Note 1: The basis of application for these reference radiographs requires a prior purchaser supplier agreement of radiographic examination attributes and classification criterion as described in Sections , , and of this standard.
Note 2: Reference radiographs previously used for this thickness range carried the designation shrinkage or C categories and by elimination of the crack and hot tear categories, except for one example of each of these discontinuity types. Reference radiographs for thicker sections may be found in Reference Radiographs and . Reference Radiographs E446 and provide some overlap of severity levels for similar discontinuity categories within the same energy level range (see , , and )., but included a now rarely used gamma source, that is, radium. The current document is also updated by inclusion of several recognized
1.2 These film reference radiographs are not intended to illustrate the types and degrees of discontinuities found in steel castings when performing digital radiography. If performing digital radiography of steel castings up to 2 in. (50.8 mm) in thickness, refer to Digital Reference Image Standard .
1.3 These reference radiographs consist of three separate volumes (see ) as follows: (I) medium voltage (nominal 250-kV) X-rays. (II) 1-MV X-rays and Iridium-192 radiation, and (III) 2-MV to 4-MV X-rays and cobalt-60 radiation. Unless otherwise specified in a purchaser supplier agreement (see ), each volume is for comparison only with production radiographs produced with radiation energy levels within the thickness range covered by this standard. Each volume consists of six categories of graded discontinuities of increasing severity level and four categories of ungraded discontinuities. Reference radiographs containing ungraded discontinuities are provided as a guide for recognition of a specific casting discontinuity type where severity levels are not needed. Following is a list of discontinuity categories, types and severity levels for the adjunct reference radiographs of this standard:
1.3.1 Category A—Gas porosity; severity levels 1 through 5.
1.3.2 Category B—Sand and slag inclusions; severity levels 1 through 5.
1.3.3 Category C—Shrinkage; 4 types:
184.108.40.206 Ca—linear shrinkage—Severity levels 1 through 5.
220.127.116.11 Cb—feathery shrinkage—Severity levels 1 through 5.
18.104.22.168 Cc—sponge shrinkage—Severity levels 1 through 5.
22.214.171.124 Cd—combinations of linear, feathery and sponge shrinkage—Severity levels 1 through 5.
1.3.4 Category D—Crack; 1 illustration.
1.3.5 Category E—Hot tear; 1 illustration.
1.3.6 Category F—Insert; 1 illustration.
1.3.7 Category G—Mottling; 1 illustration.
Note 3: The reference radiographs consist of the following:
Volume I: Medium Voltage (nominal 250 kVp) X-ray Reference Radiographs—set of 34 illustrations (nominal 5 by 7 in.) in a 15 by 17-in. ring binder.
Volume II: 1-MV X-rays and Iridium-192 Reference Radiographs—Set of 34 illustrations (nominal 5 by 7 in.) in a 15 by 17-in. ring binder.
Volume III: 2-MV to 4-MV X-rays and Cobalt-60 Reference Radiographs—Set of 34 illustrations (nominal 5 by 7 in.) in a 15 by 17-in. ring binder.
Note 4: Although Category G–Mottling is listed for all three volumes, the appearance of mottling is dependent on the level of radiation energy. Mottling appears reasonably prominent in Volume I; however, because of the higher radiation energy levels mottling may not be apparent in Volume II nor Volume III.
1.4 From time to time, there may be minor changes to the process for manufacturing of the reference radiograph adjunct materials. These changes could include changes in the films or processing chemicals used, changes in the dies or printing for the cardboard mats, etc.; however, in all cases, these changes are reviewed by the Illustration Monitoring Subcommittee and all reference radiographs are reviewed against a fixed prototype image to ensure that there are no changes to the acceptance level represented by the reference radiographs. Therefore, the adjunct reference radiographs remain valid for use with this standard regardless of the date of production or the revision level of the text standard.
1.5 Units—The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.7 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.